Journal of Visualized Experiments
Monovalent Cation Doping of CH3NH3PbI3 for Efficient Perovskite Solar Cells 1
Mojtaba Abdi-Jalebi , M. Ibrahim Dar , Aditya Sadhanala , Satyaprasad P. Senanayak , Michael Grätzel , Richard H. Friend 1
Cavendish Laboratory, University of Cambridge
Institute of Chemical Sciences and Engineering, École Polytechnique Fédérale de Lausanne
Correspondence to: Mojtaba Abdi-Jalebi at [email protected]
URL: https://www.jove.com/video/55307 DOI: doi:10.3791/55307 Keywords: Engineering, Issue 121, Monovalent cation halide, additives, CH3NH3PbI3 perovskite, doping, surface passivation Date Published: 3/19/2017 Citation: Abdi-Jalebi, M., Dar, M.I., Sadhanala, A., Senanayak, S.P., Grätzel, M., Friend, R.H. Monovalent Cation Doping of CH3NH3PbI3 for Efficient Perovskite Solar Cells. J. Vis. Exp. (121), e55307, doi:10.3791/55307 (2017).
Abstract Here, we demonstrate the incorporation of monovalent cation additives into CH3NH3PbI3 perovskite in order to adjust the optical, excitonic, and 2+ + electrical properties. The possibility of doping was investigated by adding monovalent cation halides with similar ionic radii to Pb , including Cu , + + Na , and Ag . A shift in the Fermi level and a remarkable decrease of sub-bandgap optical absorption, along with a lower energetic disorder in the perovskite, was achieved. An order-of-magnitude enhancement in the bulk hole mobility and a significant reduction of transport activation energy within an additive-based perovskite device was attained. The confluence of the aforementioned improved properties in the presence of these cations led to an enhancement in the photovoltaic parameters of the perovskite solar cell. An increase of 70 mV in open circuit voltage for 2 AgI and a 2 mA/cm improvement in photocurrent density for NaI- and CuBr-based solar cells were achieved compared to the pristine device. Our work paves the way for further improvements in the optoelectronic quality of CH3NH3PbI3 perovskite and subsequent devices. It highlights a new avenue for investigations on the role of dopant impurities in crystallization and controls the electronic defect density in perovskite structures.
Video Link The video component of this article can be found at https://www.jove.com/video/55307/
Introduction Currently, the dominant portion of the world's energy requirement (i.e., 85%) is being supplied by the combustion of oil, coal, and natural gas, 1 which facilitates global warming and has deleterious effects on our environment . Therefore, the development of CO2-neutral sources of energy is of paramount interest. Photovoltaics (PV) is an ideal energy conversion process that can meet this requirement. However, cost and efficiency, as the main obstacles to the extensive adoption of PV technology, must be improved. Emerging PV technologies based on new materials, such as perovskite solar cells (PSC), have the combination of lower cost and greater efficiency. This is achieved through the utilization of cheap 2,3,4 materials that are readily available, as well as through fast, facile, and low-energy processing routes compared to silicon-based counterparts . A remarkable improvement in the power conversion efficiency (PCE), from 3.8% to more than 22%, has been reported for hybrid organic5,6,7,8 inorganic lead halide perovskite since its first appearance in PV architecture . Such a superb performance originates from the strong light absorption with an extremely sharp band-edge, the very low energetic disorder, the weakly-bound excitons that easily dissociate into free carriers 9,10,11,12 with large diffusion lengths, and the photon recycling capability of hybrid organic-inorganic lead halide perovskite . These materials are categorized in the perovskite family, which are crystallized from organic halide and metal halide salts to form crystals in the ABX3 structure, where X is an anion and A and B are cations of different sizes (A being larger than B). Reported cations for the A site include methylammonium 13,14 (MA), formamidinium (FA), and cesium (Cs); a combination of these cations shows the highest performance . Furthermore, the main candidate for the divalent cation in the B site is lead, which can be replaced by tin; the bandgap can be successfully red-shifted to over 1,000 15 nm in a lead-tin mixed perovskite . Similarly, the X-site occupants have been studied extensively, where a mixture of iodide (I) and bromide 16,17 (Br) were introduced as the main candidates . Therefore, it is highly plausible to manipulate the structural, morphological, and optoelectronic properties of perovskites by altering their chemical composition. Despite the fact that the enhanced crystalline quality and the macroscopic uniformity of the perovskite film are key parameters to achieve efficient 18 devices , the impact of the boundaries between the polycrystalline domains, the origin and role of electronic defects in the perovskite absorbers, and the role of the charge collection layers upon loss processes in the perovskite solar cells are not yet well understood. Regarding the nature of electronic defects in the perovskite structure, it has been reported that many of the defects, such as I or Pb vacancies, result in states that are very close to or within the continuum of states in the conduction and valence bands, which might have a negative electronic impact on the 19 photovoltaic devices . In addition, a strong covalent bonding interaction between lead cations and iodide anions in the perovskite plane may lead to the existence of intrinsic defects (e.g., under-coordinated Pb dimers and I trimers), which could create sites within the band-edge that act 20 as charge recombination centers during the operation of the device . +
Here, we investigate the impact of doping CH3NH3PbI3 perovskite with monovalent cation halides, including Na , Cu , and Ag , lower-valence 2+ metal ions than Pb . We therefore incorporate these cations through the addition of a rational amount of their halide-based salts (e.g., NaI, 2+ CuBr, CuI, and AgI) into the perovskite precursor solution. These cations have ionic radii similar to Pb , so substitutional doping within the Copyright © 2017 Creative Commons Attribution-NonCommercial-NoDerivs 3.0 Unported License
March 2017 | 121 | e55307 | Page 1 of 9
Journal of Visualized Experiments
crystal is probable. We have shown that the presence of these cations strongly affects both the morphology and coverage of the perovskite layer. + + In addition, the presence of these cations (e.g., Na and Ag ) has been confirmed by X-ray photoelectron spectroscopy (XPS), and a significant change in the Fermi level of perovskite was measured by Kelvin probe force microscopy (KPFM). By incorporating these cations into sequentially deposited perovskite solar cells, we achieved an improvement in the photovoltaic efficiency of PSC (15.6% compare to 14%). Therefore, it is very essential to enhance the structural and optoelectronic properties of the absorber layer (e.g., perovskite) in solar cell architecture to maximize the charge transport and to passivate the surface traps in order to reach the highest PV performance.
1. Synthesis and Deposition of Pristine and Additive-based CH3NH3PbI3 NOTE: All the solutions were prepared inside an argon glove box under moisture- and oxygen-controlled conditions (H2O level: